Home >
Documents >
1 IIII mmmm pppp eeee rrrr ffff eeee cccc tttt iiii oooo nnnn ssss IIII nnnn S S S S oooo llll iiii...

Date post: | 05-Jan-2016 |

Category: |
## Documents |

Author: | mabel-hunter |

View: | 277 times |

Download: | 1 times |

Share this document with a friend

Embed Size (px)

of 82
/82

1 Imperfectio nsIn Solids Chapter 5 Chapter 5

Transcript

Slide 1Use metals as Prototypical Example

How the number and type of defects Can be varied and controlled

How defects affect material properties

Determine if “Defects” are

*

Point defects - Imperfections, such as vacancies, that are located typically at one (in some cases a few) sites in the crystal.

Extended defects - Defects that involve several atoms/ions and thus occur over a finite volume of the crystalline material (e.g., dislocations, stacking faults, etc.).

Vacancy - An atom or an ion missing from its regular crystallographic site.

Interstitial defect - A point defect produced when an atom is placed into the crystal at a site that is normally not a lattice point.

Substitutional defect - A point defect produced when an atom is removed from a regular lattice point and replaced with a different atom, usually of a different size.

Section 5.1

Point Defects

Self-Interstitial “Extra” Atom “Squeezed

into the Lattice Structure

*

Figure 5.1 Point defects: (a) vacancy, (b) interstitial atom, (c) small substitutional atom, (d) large substitutional atom, (e) Frenkel defect, (f) Schottky defect. All of these defects disrupt the perfect arrangement of the surrounding atoms.

(c) 2003 Brooks/Cole Publishing / Thomson Learning

*

k =

Recall The Defect Density Eqn

Take the ln of Eqn

This form of a Negative Exponential is called an Arrhenius Relation

Svante Arrhenius: 1859-1927, Chem Nobel 1903

This of the form

RePlot in Linear Form

Qv Vacancies

Qi Interstitials

*

Now apply the Arrhenius Relation @1000 ºC

275 ppm Vacancy Rate

*

Calculate the concentration of vacancies in copper at room temperature (25oC). What temperature will be needed to heat treat copper such that the concentration of vacancies produced will be 1000 times more than the equilibrium concentration of vacancies at room temperature? Assume that 20,000 cal are required to produce a mole of vacancies in copper.

Example 5.1 SOLUTION

The lattice parameter of FCC copper is 0.36151 nm. The basis is 1, therefore, the number of copper atoms, or lattice points, per cm3 is:

Example 5.1 The Effect of Temperature on Vacancy Concentrations

*

At room temperature, T = 25 + 273 = 298 K:

*

Determine the number of vacancies needed for a BCC iron crystal to have a density of 7.87 g/cm3. The lattice parameter of the iron is 2.866 10-8 cm.

Example 5.2 SOLUTION

The expected theoretical density of iron can be calculated from the lattice parameter and the atomic mass.

Example 5.2 Vacancy Concentrations in Iron

*

Example 5.2 SOLUTION (Continued)

Let’s calculate the number of iron atoms and vacancies that would be present in each unit cell for the required density of 7.87 g/cm3:

*

In FCC iron, carbon atoms are located at octahedral sites at the center of each edge of the unit cell (1/2, 0, 0) and at the center of the unit cell (1/2, 1/2, 1/2). In BCC iron, carbon atoms enter tetrahedral sites, such as 1/4, 1/2, 0. The lattice parameter is 0.3571 nm for FCC iron and 0.2866 nm for BCC iron. Assume that carbon atoms have a radius of 0.071 nm. (1) Would we expect a greater distortion of the crystal by an interstitial carbon atom in FCC or BCC iron? (2) What would be the atomic percentage of carbon in each type of iron if all the interstitial sites were filled?

Homework: Example 5.3 Sites for Carbon in Iron

*

Figure 5.3 (a) The location of the ¼, ½, 0 interstitial site in BCC metals, showing the arrangement of the normal atoms and the interstitial atom (b) ½, 0, 0 site in FCC metals, (for Example 5.3). (c) Edge centers and cube centers are some of the interstitial sites in the FCC structure (Example 5.3).

(c) 2003 Brooks/Cole Publishing / Thomson Learning

*

Three separate samples of germanium (Ge) crystals contain small concentrations of either silicon (Si), arsenic (As), or boron (B) as dopants. Based on the valence of these elements, what type of semiconductivity is expected from these materials? Assume that these elements will occupy Ge sites.

Example 5.4 SOLUTION

When Si is added to Ge, silicon atoms can form four bonds with neighboring Ge atoms. As a result, there is no need to donate or accept an electron. The resultant material then does not show either ‘‘n-type’’ or ‘‘p-type’’ conductivity.

When we add As, we expect n-type conductivity since each As atom brings in five valence electrons.

When we add small concentrations of B to Ge we expect p-type conductivity for the resultant material, since B has a valence of 3.

Example 5.4 Dopants in Germanium Semiconductor

*

Interstitialcy - A point defect caused when a ‘‘normal’’ atom occupies an interstitial site in the crystal.

Frenkel defect - A pair of point defects produced when an ion moves to create an interstitial site, leaving behind a vacancy.

Schottky defect - A point defect in ionically bonded materials. In order to maintain a neutral charge, a stoichiometric number of cation and anion vacancies must form.

KrÖger-Vink notation - A system used to indicate point defects in materials. The main body of the notation indicates the type of defect or the element involved.

Section 5.2 Other Point Defects

*

Figure 5.3 When a divalent cation replaces a monovalent cation, a second monovalent cation must also be removed, creating a vacancy.

(c) 2003 Brooks/Cole Publishing / Thomson Learning

*

Write the appropriate defect reactions for (1) incorporation of magnesium oxide (MgO) in nickel oxide (NiO), and (2) formation of a Schottky defect in alumina (Al2O3).

Example 5.5 SOLUTION

1. MgO is the guest and NiO is the host material. We will assume that Mg+2 ions will occupy Ni+2 sites and oxygen anions from MgO will occupy O-2 sites of NiO.

Example 5.5 Application of the Kröger-Vink Notation

*

Write the appropriate defect reactions for the incorporation of calcium oxide (CaO) in zirconia (ZrO2) using the Kröger-Vink notation.

Example 5.6 SOLUTION

We will assume that Ca+2 will occupy Zr+4 sites. If we send one Ca+2 to Zr+4, the site will have an effective negative charge of -2 (instead of having a charge of +4 we have a charge of +2). We have used one Zr+4 site and site balance would require us to utilize two oxygen sites. We can send one O-2 from CaO to one of the O-2 sites in ZrO2. The other oxygen site must be used and since mass balance must also be maintained we will have to keep this site vacant.

*

Two outcomes if impurity (B) added to host (A)

Solid solution of B in A (i.e., random dist. of point defects)

Solid solution of B in A plus particles of a NEW PHASE (usually for a larger amount of B)

OR

Composition/Concentration

Composition Amount of impurity/solute (B) and host/solvent (A) in the SYSTEM.

Two Forms

Weight-%

Where

Atom/Mol %

Where

*

Dislocation - A line imperfection in a crystalline material.

Screw dislocation - A dislocation produced by skewing a crystal so that one atomic plane produces a spiral ramp about the dislocation.

Edge dislocation - A dislocation introduced into the crystal by adding an ‘‘extra half plane’’ of atoms.

Mixed dislocation - A dislocation that contains partly edge components and partly screw components.

Slip - Deformation of a metallic material by the movement of dislocations through the crystal.

Section 5.3 Dislocations

First PREDICTED as defects in crystals since theoretical strength calculations (due to multibond breaking) were far too low as compared to experiments

later invention of the Transmission Electron Microscope (TEM) PROVED their Existence

deformed

steel

(40,000X)

* CREATED during deformation

*

Figure 5.4 the perfect crystal (a) is cut and sheared one atom spacing, (b) and (c). The line along which shearing occurs is a screw dislocation. A Burgers vector b is required to close a loop of equal atom spacings around the screw dislocation.

(c) 2003 Brooks/Cole Publishing / Thomson Learning

*

*

*

*

*

linear defect

moves in response to shear stress and results in bulk atomic movement

cause of slip between crystal planes when they move

*

*

Dislocations Move Thru the Crystal in Response to Shear Force

Result in Net atomic Movement or DEFORMATION

*

A sketch of a dislocation in magnesium oxide (MgO), which has the sodium chloride crystal structure and a lattice parameter of 0.396 nm, is shown in Figure 5.9. Determine the length of the Burgers vector.

Example 5.7 Dislocations in Ceramic Materials

*

Example 5.7 SOLUTION

In Figure 5.9, we begin a clockwise loop around the dislocation at point x, then move equal atom spacings to finish at point y. The vector b is the Burgers vector. Because b is a [110] direction, it must be perpendicular to {110} planes. The length of b is the distance between two adjacent (110) planes. From Equation 3-7,

Note that this formula for calculating the magnitude of the Burgers vector will not work for non-cubic systems. It is better to consider the magntiude of the Burgers vector

*

Homework: Example 5.8 Burgers Vector Calculation

Figure 5.10 (a) Burgers vector for FCC copper. (b) The atom locations on a (110) plane in a BCC unit cell (for example 5.8 and 5.9, respectively)

(c) 2003 Brooks/Cole Publishing / Thomson Learning

*

The planar density of the (112) plane in BCC iron is 9.94 1014 atoms/cm2. Calculate (1) the planar density of the (110) plane and (2) the interplanar spacings for both the (112) and (110) planes. On which plane would slip normally occur?

Homework: Example 5.9 Identification of Preferred Slip Planes

Figure 5.10 (a) Burgers vector for FCC copper. (b) The atom locations on a (110) plane in a BCC unit cell (for example 5.8 and 5.9, respectively)

(c) 2003 Brooks/Cole Publishing / Thomson Learning

*

Etch pits - Tiny holes created at areas where dislocations meet the surface. These are used to examine the presence and number density of dislocations.

Slip line - A visible line produced at the surface of a metallic material by the presence of several thousand dislocations.

Slip band - Collection of many slip lines, often easily visible.

Section 5.4 Observing Dislocations

*

Figure 5.11 A sketch illustrating dislocations, slip planes, and etch pit locations. (Source: Adapted from Physical Metallurgy Principles, Third Edition, by R.E. Reed-Hill and R. Abbaschian, p. 92, Figs. 4-7 and 4-8. Copyright (c) 1992 Brooks/Cole Thomson Learning. Adapted by permission.)

(c) 2003 Brooks/Cole Publishing / Thomson Learning

*

*

Figure 5.13 Electron photomicrographs of dislocations in Ti3Al: (a) Dislocation pileups (x26,500). (b) Micrograph at x 100 showing slip lines and grain boundaries in AI. (c) Schematic of slip bands development.

(c) 2003 Brooks/Cole Publishing / Thomson Learning

(c) 2003 Brooks/Cole Publishing / Thomson Learning

*

Plastic deformation refers to irreversible deformation or change in shape that occurs when the force or stress that caused it is removed.

Elastic deformation - Deformation that is fully recovered when the stress causing it is removed.

Dislocation density - The total length of dislocation line per cubic centimeter in a material.

Section 5.5 Significance of Dislocations

*

Some Macro-Scale Examples

Solid Surfaces (Edges)

Source of “Surface Energy” in Units of J/sq-m

Stacking Faults – When atom-Plane Stacking Pattern is Not as Expected

Phase Boundaries – InterFace Between Different Xtal Structures

*

Orientation across them

IMPEDE dislocation motion

Typically Reduce Material Strength thru

Grain-Boundary Tearing

~ 8cm

Section 5.6 Schmid’s Law

Schmid’s law -The relationship between shear stress, the applied stress, and the orientation of the slip system—that is,

*

Slip can occur in some ceramics and polymers

Useful for understanding the mechanical behavior of materials

Slip explains why the strength of metals is much lower than predicted from the metalic bond

Slip provides ductility of metals, so that metal is not brittle

*

Figure 5.14 (a) A resolved shear stress τ is produced on a slip system. (Note: (ø + λ) does not have to be 90°.) (b) Movement of dislocations on the slip system deforms the material. (c) Resolving the force.

*

Apply the Schmid’s law for a situation in which the single crystal is at an orientation so that the slip plane is perpendicular to the applied tensile stress.

Example 5.10 Calculation of Resolved Shear Stress

Figure 15.15 When the slip plane is perpendicular to the applied stress σ, the angle λ is 90° and no shear stress is resolved.

(c) 2003 Brooks/Cole Publishing / Thomson Learning

*

Example 5.10 SOLUTION

Suppose the slip plane is perpendicular to the applied stress σ, as in Figure 5.15. Then, ø = 0o, λ = 90o, cos λ = 0, and therefore r = 0. As noted before, the angles ø and λ can but do not always add up to 90o.

*

We wish to produce a rod composed of a single crystal of pure aluminum, which has a critical resolved shear stress of 148 psi. We would like to orient the rod in such a manner that, when an axial stress of 500 psi is applied, the rod deforms by slip in a 45o direction to the axis of the rod and actuates a sensor that detects the overload. Design the rod and a method by which it might be produced.

Example 5.11 SOLUTION

Dislocations begin to move when the resolved shear stress τr equals the critical resolved shear stress, 148 psi. From Schmid’s law:

τr = σ cos λ cos ø; or

148 psi = (500 psi) cos λ cos ø

Example 5.11 Design of a Single Crystal Casting Process

*

Example 5.11 SOLUTION (Continued)

Because we wish slip to occur at a 45o angle to the axis of the rod, λ = 45o, and:

Therefore, we must produce a rod that is oriented such that λ = 45o and ø = 65.2o. Note that ø and λ do not add to 90o.

*

Critical Resolved Shear Stress: The shear stress required to cause a dislocation to move and cause slip.

Number of Slip Systems

Cross-slip - A change in the slip system of a dislocation.

Section 5.7 Influence of Crystal Structure

*

*

A single crystal of magnesium (Mg), which has a HCP crystal structure, can be stretched into a ribbon-like shape four to six times its original length. However, polycrystalline Mg and other metals with a HCP structure show limited ductilities. Use the values of critical resolved shear stress for metals with different crystal structures and the nature of deformation in polycrystalline materials to explain this observation.

*

*

Example 5.12 SOLUTION

From Table 4-2, we note that for HCP metals such as Mg, the critical resolved shear stress is low (50–100 psi). We also note that slip in HCP metals will occur readily on the basal plane—the primary slip plane. When a single crystal is deformed, assuming the basal plane is suitably oriented with applied stress, a very large deformation can occur. This explains why single crystal Mg can be stretched into a ribbon four to six times the original size.

*

Since Most Solid Materials are Opaque, MicroScope Uses REFLECTED Light

These METALLOGRAHPIC MScopes do NOT have a CONDENSOR Lens

*

Typical Values

Objects Closer Together than This Cannot Be Separated

Mtrue 200

sometimes use chemical etch

are more susceptible to etching; may be revealed as

dark lines

Where

Electron Microscopy

For much greater resolution, use BEAM OF ELECTRONS rather that light radiation

Transmission Electron Microscopy (TEM):

tiny probe with tiny tip rasters surface

topographical map on atomic scale

Will See on SEM & AFM on

CE&A Tour

Surface defects - Imperfections, such as grain boundaries, that form a two-dimensional plane within the crystal.

Hall-Petch equation - The relationship between yield strength and grain size in a metallic material—that is,

ASTM grain size number (n) - A measure of the size of the grains in a crystalline material obtained by counting the number of grains per square inch a magnification 100.

*

*

Figure 5.17 The effect of grain size on the yield strength of steel at room temperature.

(c) 2003 Brooks/Cole Publishing / Thomson Learning

*

The yield strength of mild steel with an average grain size of 0.05 mm is 20,000 psi. The yield stress of the same steel with a grain size of 0.007 mm is 40,000 psi. What will be the average grain size of the same steel with a yield stress of 30,000 psi? Assume the Hall-Petch equation is valid and that changes in the observed yield stress are due to changes in dislocation density.

Example 5.13 SOLUTION

Example 5.13 Design of a Mild Steel

Thus, for a grain size of 0.05 mm the yield stress is

20 6.895 MPa = 137.9 MPa.

(Note:1,000 psi = 6.895 MPa). Using the Hall-Petch equation

*

Example 5.13 SOLUTION (Continued)

For the grain size of 0.007 mm, the yield stress is 40 6.895 MPa = 275.8 MPa. Therefore, again using the Hall-Petch equation:

Solving these two equations K = 18.43 MPa-mm1/2, and σ0 = 55.5 MPa. Now we have the Hall-Petch equation as

σy = 55.5 + 18.43 d-1/2

*

*

Suppose we count 16 grains per square inch in a photomicrograph taken at magnification 250. What is the ASTM grain size number?

Example 5.14 SOLUTION

If we count 16 grains per square inch at magnification 250, then at magnification 100 we must have:

N = (250/100)2 (16) = 100 grains/in.2 = 2n-1

Log 100 = (n – 1) log 2

2 = (n – 1)(0.301)

*

Figure 5.19 The small angle grain boundary is produced by an array of dislocations, causing an angular mismatch θ between lattices on either side of the boundary.

(c) 2003 Brooks/Cole Publishing / Thomson Learning

*

Figure 5.20 Application of a stress to the perfect crystal (a) may cause a displacement of the atoms, (b) causing the formation of a twin. Note that the crystal has deformed as a result of twinning.

(c) 2003 Brooks/Cole Publishing / Thomson Learning

*

Figure 5.20 (c) A micrograph of twins within a grain of brass (x250).

(c) 2003 Brooks/Cole Publishing / Thomson Learning

*

*

*

Effect on Mechanical Properties via Control of the Slip Process

Strain Hardening

Solid-Solution Strengthening

Grain-Size Strengthening

Section 5.9 Importance of Defects

*

Figure 5.22 If the dislocation at point A moves to the left, it is blocked by the point defect. If the dislocation moves to the right, it interacts with the disturbed lattice near the second dislocation at point B. If the dislocation moves farther to the right, it is blocked by a grain boundary.

*

We would like to produce a bracket to hold ceramic bricks in place in a heat-treating furnace. The bracket should be strong, should possess some ductility so that it bends rather than fractures if overloaded, and should maintain most of its strength up to 600oC. Design the material for this bracket, considering the various crystal imperfections as the strengthening mechanism.

Example 5.15 SOLUTION

In order to serve up to 600oC, the bracket should not be produced from a polymer material. Instead, a metal or ceramic would be considered.

Example 5.15 Design/Materials Selection for a Stable Structure

*

Example 5.15 SOLUTION (Continued)

*

*

Figure 5.24 The microstructure of BMT ceramics obtained by compaction and sintering of BMT powders. (Courtesy of H. Shirey.)

kT

Q

D

D

e

N

N

How the number and type of defects Can be varied and controlled

How defects affect material properties

Determine if “Defects” are

*

Point defects - Imperfections, such as vacancies, that are located typically at one (in some cases a few) sites in the crystal.

Extended defects - Defects that involve several atoms/ions and thus occur over a finite volume of the crystalline material (e.g., dislocations, stacking faults, etc.).

Vacancy - An atom or an ion missing from its regular crystallographic site.

Interstitial defect - A point defect produced when an atom is placed into the crystal at a site that is normally not a lattice point.

Substitutional defect - A point defect produced when an atom is removed from a regular lattice point and replaced with a different atom, usually of a different size.

Section 5.1

Point Defects

Self-Interstitial “Extra” Atom “Squeezed

into the Lattice Structure

*

Figure 5.1 Point defects: (a) vacancy, (b) interstitial atom, (c) small substitutional atom, (d) large substitutional atom, (e) Frenkel defect, (f) Schottky defect. All of these defects disrupt the perfect arrangement of the surrounding atoms.

(c) 2003 Brooks/Cole Publishing / Thomson Learning

*

k =

Recall The Defect Density Eqn

Take the ln of Eqn

This form of a Negative Exponential is called an Arrhenius Relation

Svante Arrhenius: 1859-1927, Chem Nobel 1903

This of the form

RePlot in Linear Form

Qv Vacancies

Qi Interstitials

*

Now apply the Arrhenius Relation @1000 ºC

275 ppm Vacancy Rate

*

Calculate the concentration of vacancies in copper at room temperature (25oC). What temperature will be needed to heat treat copper such that the concentration of vacancies produced will be 1000 times more than the equilibrium concentration of vacancies at room temperature? Assume that 20,000 cal are required to produce a mole of vacancies in copper.

Example 5.1 SOLUTION

The lattice parameter of FCC copper is 0.36151 nm. The basis is 1, therefore, the number of copper atoms, or lattice points, per cm3 is:

Example 5.1 The Effect of Temperature on Vacancy Concentrations

*

At room temperature, T = 25 + 273 = 298 K:

*

Determine the number of vacancies needed for a BCC iron crystal to have a density of 7.87 g/cm3. The lattice parameter of the iron is 2.866 10-8 cm.

Example 5.2 SOLUTION

The expected theoretical density of iron can be calculated from the lattice parameter and the atomic mass.

Example 5.2 Vacancy Concentrations in Iron

*

Example 5.2 SOLUTION (Continued)

Let’s calculate the number of iron atoms and vacancies that would be present in each unit cell for the required density of 7.87 g/cm3:

*

In FCC iron, carbon atoms are located at octahedral sites at the center of each edge of the unit cell (1/2, 0, 0) and at the center of the unit cell (1/2, 1/2, 1/2). In BCC iron, carbon atoms enter tetrahedral sites, such as 1/4, 1/2, 0. The lattice parameter is 0.3571 nm for FCC iron and 0.2866 nm for BCC iron. Assume that carbon atoms have a radius of 0.071 nm. (1) Would we expect a greater distortion of the crystal by an interstitial carbon atom in FCC or BCC iron? (2) What would be the atomic percentage of carbon in each type of iron if all the interstitial sites were filled?

Homework: Example 5.3 Sites for Carbon in Iron

*

Figure 5.3 (a) The location of the ¼, ½, 0 interstitial site in BCC metals, showing the arrangement of the normal atoms and the interstitial atom (b) ½, 0, 0 site in FCC metals, (for Example 5.3). (c) Edge centers and cube centers are some of the interstitial sites in the FCC structure (Example 5.3).

(c) 2003 Brooks/Cole Publishing / Thomson Learning

*

Three separate samples of germanium (Ge) crystals contain small concentrations of either silicon (Si), arsenic (As), or boron (B) as dopants. Based on the valence of these elements, what type of semiconductivity is expected from these materials? Assume that these elements will occupy Ge sites.

Example 5.4 SOLUTION

When Si is added to Ge, silicon atoms can form four bonds with neighboring Ge atoms. As a result, there is no need to donate or accept an electron. The resultant material then does not show either ‘‘n-type’’ or ‘‘p-type’’ conductivity.

When we add As, we expect n-type conductivity since each As atom brings in five valence electrons.

When we add small concentrations of B to Ge we expect p-type conductivity for the resultant material, since B has a valence of 3.

Example 5.4 Dopants in Germanium Semiconductor

*

Interstitialcy - A point defect caused when a ‘‘normal’’ atom occupies an interstitial site in the crystal.

Frenkel defect - A pair of point defects produced when an ion moves to create an interstitial site, leaving behind a vacancy.

Schottky defect - A point defect in ionically bonded materials. In order to maintain a neutral charge, a stoichiometric number of cation and anion vacancies must form.

KrÖger-Vink notation - A system used to indicate point defects in materials. The main body of the notation indicates the type of defect or the element involved.

Section 5.2 Other Point Defects

*

Figure 5.3 When a divalent cation replaces a monovalent cation, a second monovalent cation must also be removed, creating a vacancy.

(c) 2003 Brooks/Cole Publishing / Thomson Learning

*

Write the appropriate defect reactions for (1) incorporation of magnesium oxide (MgO) in nickel oxide (NiO), and (2) formation of a Schottky defect in alumina (Al2O3).

Example 5.5 SOLUTION

1. MgO is the guest and NiO is the host material. We will assume that Mg+2 ions will occupy Ni+2 sites and oxygen anions from MgO will occupy O-2 sites of NiO.

Example 5.5 Application of the Kröger-Vink Notation

*

Write the appropriate defect reactions for the incorporation of calcium oxide (CaO) in zirconia (ZrO2) using the Kröger-Vink notation.

Example 5.6 SOLUTION

We will assume that Ca+2 will occupy Zr+4 sites. If we send one Ca+2 to Zr+4, the site will have an effective negative charge of -2 (instead of having a charge of +4 we have a charge of +2). We have used one Zr+4 site and site balance would require us to utilize two oxygen sites. We can send one O-2 from CaO to one of the O-2 sites in ZrO2. The other oxygen site must be used and since mass balance must also be maintained we will have to keep this site vacant.

*

Two outcomes if impurity (B) added to host (A)

Solid solution of B in A (i.e., random dist. of point defects)

Solid solution of B in A plus particles of a NEW PHASE (usually for a larger amount of B)

OR

Composition/Concentration

Composition Amount of impurity/solute (B) and host/solvent (A) in the SYSTEM.

Two Forms

Weight-%

Where

Atom/Mol %

Where

*

Dislocation - A line imperfection in a crystalline material.

Screw dislocation - A dislocation produced by skewing a crystal so that one atomic plane produces a spiral ramp about the dislocation.

Edge dislocation - A dislocation introduced into the crystal by adding an ‘‘extra half plane’’ of atoms.

Mixed dislocation - A dislocation that contains partly edge components and partly screw components.

Slip - Deformation of a metallic material by the movement of dislocations through the crystal.

Section 5.3 Dislocations

First PREDICTED as defects in crystals since theoretical strength calculations (due to multibond breaking) were far too low as compared to experiments

later invention of the Transmission Electron Microscope (TEM) PROVED their Existence

deformed

steel

(40,000X)

* CREATED during deformation

*

Figure 5.4 the perfect crystal (a) is cut and sheared one atom spacing, (b) and (c). The line along which shearing occurs is a screw dislocation. A Burgers vector b is required to close a loop of equal atom spacings around the screw dislocation.

(c) 2003 Brooks/Cole Publishing / Thomson Learning

*

*

*

*

*

linear defect

moves in response to shear stress and results in bulk atomic movement

cause of slip between crystal planes when they move

*

*

Dislocations Move Thru the Crystal in Response to Shear Force

Result in Net atomic Movement or DEFORMATION

*

A sketch of a dislocation in magnesium oxide (MgO), which has the sodium chloride crystal structure and a lattice parameter of 0.396 nm, is shown in Figure 5.9. Determine the length of the Burgers vector.

Example 5.7 Dislocations in Ceramic Materials

*

Example 5.7 SOLUTION

In Figure 5.9, we begin a clockwise loop around the dislocation at point x, then move equal atom spacings to finish at point y. The vector b is the Burgers vector. Because b is a [110] direction, it must be perpendicular to {110} planes. The length of b is the distance between two adjacent (110) planes. From Equation 3-7,

Note that this formula for calculating the magnitude of the Burgers vector will not work for non-cubic systems. It is better to consider the magntiude of the Burgers vector

*

Homework: Example 5.8 Burgers Vector Calculation

Figure 5.10 (a) Burgers vector for FCC copper. (b) The atom locations on a (110) plane in a BCC unit cell (for example 5.8 and 5.9, respectively)

(c) 2003 Brooks/Cole Publishing / Thomson Learning

*

The planar density of the (112) plane in BCC iron is 9.94 1014 atoms/cm2. Calculate (1) the planar density of the (110) plane and (2) the interplanar spacings for both the (112) and (110) planes. On which plane would slip normally occur?

Homework: Example 5.9 Identification of Preferred Slip Planes

Figure 5.10 (a) Burgers vector for FCC copper. (b) The atom locations on a (110) plane in a BCC unit cell (for example 5.8 and 5.9, respectively)

(c) 2003 Brooks/Cole Publishing / Thomson Learning

*

Etch pits - Tiny holes created at areas where dislocations meet the surface. These are used to examine the presence and number density of dislocations.

Slip line - A visible line produced at the surface of a metallic material by the presence of several thousand dislocations.

Slip band - Collection of many slip lines, often easily visible.

Section 5.4 Observing Dislocations

*

Figure 5.11 A sketch illustrating dislocations, slip planes, and etch pit locations. (Source: Adapted from Physical Metallurgy Principles, Third Edition, by R.E. Reed-Hill and R. Abbaschian, p. 92, Figs. 4-7 and 4-8. Copyright (c) 1992 Brooks/Cole Thomson Learning. Adapted by permission.)

(c) 2003 Brooks/Cole Publishing / Thomson Learning

*

*

Figure 5.13 Electron photomicrographs of dislocations in Ti3Al: (a) Dislocation pileups (x26,500). (b) Micrograph at x 100 showing slip lines and grain boundaries in AI. (c) Schematic of slip bands development.

(c) 2003 Brooks/Cole Publishing / Thomson Learning

(c) 2003 Brooks/Cole Publishing / Thomson Learning

*

Plastic deformation refers to irreversible deformation or change in shape that occurs when the force or stress that caused it is removed.

Elastic deformation - Deformation that is fully recovered when the stress causing it is removed.

Dislocation density - The total length of dislocation line per cubic centimeter in a material.

Section 5.5 Significance of Dislocations

*

Some Macro-Scale Examples

Solid Surfaces (Edges)

Source of “Surface Energy” in Units of J/sq-m

Stacking Faults – When atom-Plane Stacking Pattern is Not as Expected

Phase Boundaries – InterFace Between Different Xtal Structures

*

Orientation across them

IMPEDE dislocation motion

Typically Reduce Material Strength thru

Grain-Boundary Tearing

~ 8cm

Section 5.6 Schmid’s Law

Schmid’s law -The relationship between shear stress, the applied stress, and the orientation of the slip system—that is,

*

Slip can occur in some ceramics and polymers

Useful for understanding the mechanical behavior of materials

Slip explains why the strength of metals is much lower than predicted from the metalic bond

Slip provides ductility of metals, so that metal is not brittle

*

Figure 5.14 (a) A resolved shear stress τ is produced on a slip system. (Note: (ø + λ) does not have to be 90°.) (b) Movement of dislocations on the slip system deforms the material. (c) Resolving the force.

*

Apply the Schmid’s law for a situation in which the single crystal is at an orientation so that the slip plane is perpendicular to the applied tensile stress.

Example 5.10 Calculation of Resolved Shear Stress

Figure 15.15 When the slip plane is perpendicular to the applied stress σ, the angle λ is 90° and no shear stress is resolved.

(c) 2003 Brooks/Cole Publishing / Thomson Learning

*

Example 5.10 SOLUTION

Suppose the slip plane is perpendicular to the applied stress σ, as in Figure 5.15. Then, ø = 0o, λ = 90o, cos λ = 0, and therefore r = 0. As noted before, the angles ø and λ can but do not always add up to 90o.

*

We wish to produce a rod composed of a single crystal of pure aluminum, which has a critical resolved shear stress of 148 psi. We would like to orient the rod in such a manner that, when an axial stress of 500 psi is applied, the rod deforms by slip in a 45o direction to the axis of the rod and actuates a sensor that detects the overload. Design the rod and a method by which it might be produced.

Example 5.11 SOLUTION

Dislocations begin to move when the resolved shear stress τr equals the critical resolved shear stress, 148 psi. From Schmid’s law:

τr = σ cos λ cos ø; or

148 psi = (500 psi) cos λ cos ø

Example 5.11 Design of a Single Crystal Casting Process

*

Example 5.11 SOLUTION (Continued)

Because we wish slip to occur at a 45o angle to the axis of the rod, λ = 45o, and:

Therefore, we must produce a rod that is oriented such that λ = 45o and ø = 65.2o. Note that ø and λ do not add to 90o.

*

Critical Resolved Shear Stress: The shear stress required to cause a dislocation to move and cause slip.

Number of Slip Systems

Cross-slip - A change in the slip system of a dislocation.

Section 5.7 Influence of Crystal Structure

*

*

A single crystal of magnesium (Mg), which has a HCP crystal structure, can be stretched into a ribbon-like shape four to six times its original length. However, polycrystalline Mg and other metals with a HCP structure show limited ductilities. Use the values of critical resolved shear stress for metals with different crystal structures and the nature of deformation in polycrystalline materials to explain this observation.

*

*

Example 5.12 SOLUTION

From Table 4-2, we note that for HCP metals such as Mg, the critical resolved shear stress is low (50–100 psi). We also note that slip in HCP metals will occur readily on the basal plane—the primary slip plane. When a single crystal is deformed, assuming the basal plane is suitably oriented with applied stress, a very large deformation can occur. This explains why single crystal Mg can be stretched into a ribbon four to six times the original size.

*

Since Most Solid Materials are Opaque, MicroScope Uses REFLECTED Light

These METALLOGRAHPIC MScopes do NOT have a CONDENSOR Lens

*

Typical Values

Objects Closer Together than This Cannot Be Separated

Mtrue 200

sometimes use chemical etch

are more susceptible to etching; may be revealed as

dark lines

Where

Electron Microscopy

For much greater resolution, use BEAM OF ELECTRONS rather that light radiation

Transmission Electron Microscopy (TEM):

tiny probe with tiny tip rasters surface

topographical map on atomic scale

Will See on SEM & AFM on

CE&A Tour

Surface defects - Imperfections, such as grain boundaries, that form a two-dimensional plane within the crystal.

Hall-Petch equation - The relationship between yield strength and grain size in a metallic material—that is,

ASTM grain size number (n) - A measure of the size of the grains in a crystalline material obtained by counting the number of grains per square inch a magnification 100.

*

*

Figure 5.17 The effect of grain size on the yield strength of steel at room temperature.

(c) 2003 Brooks/Cole Publishing / Thomson Learning

*

The yield strength of mild steel with an average grain size of 0.05 mm is 20,000 psi. The yield stress of the same steel with a grain size of 0.007 mm is 40,000 psi. What will be the average grain size of the same steel with a yield stress of 30,000 psi? Assume the Hall-Petch equation is valid and that changes in the observed yield stress are due to changes in dislocation density.

Example 5.13 SOLUTION

Example 5.13 Design of a Mild Steel

Thus, for a grain size of 0.05 mm the yield stress is

20 6.895 MPa = 137.9 MPa.

(Note:1,000 psi = 6.895 MPa). Using the Hall-Petch equation

*

Example 5.13 SOLUTION (Continued)

For the grain size of 0.007 mm, the yield stress is 40 6.895 MPa = 275.8 MPa. Therefore, again using the Hall-Petch equation:

Solving these two equations K = 18.43 MPa-mm1/2, and σ0 = 55.5 MPa. Now we have the Hall-Petch equation as

σy = 55.5 + 18.43 d-1/2

*

*

Suppose we count 16 grains per square inch in a photomicrograph taken at magnification 250. What is the ASTM grain size number?

Example 5.14 SOLUTION

If we count 16 grains per square inch at magnification 250, then at magnification 100 we must have:

N = (250/100)2 (16) = 100 grains/in.2 = 2n-1

Log 100 = (n – 1) log 2

2 = (n – 1)(0.301)

*

Figure 5.19 The small angle grain boundary is produced by an array of dislocations, causing an angular mismatch θ between lattices on either side of the boundary.

(c) 2003 Brooks/Cole Publishing / Thomson Learning

*

Figure 5.20 Application of a stress to the perfect crystal (a) may cause a displacement of the atoms, (b) causing the formation of a twin. Note that the crystal has deformed as a result of twinning.

(c) 2003 Brooks/Cole Publishing / Thomson Learning

*

Figure 5.20 (c) A micrograph of twins within a grain of brass (x250).

(c) 2003 Brooks/Cole Publishing / Thomson Learning

*

*

*

Effect on Mechanical Properties via Control of the Slip Process

Strain Hardening

Solid-Solution Strengthening

Grain-Size Strengthening

Section 5.9 Importance of Defects

*

Figure 5.22 If the dislocation at point A moves to the left, it is blocked by the point defect. If the dislocation moves to the right, it interacts with the disturbed lattice near the second dislocation at point B. If the dislocation moves farther to the right, it is blocked by a grain boundary.

*

We would like to produce a bracket to hold ceramic bricks in place in a heat-treating furnace. The bracket should be strong, should possess some ductility so that it bends rather than fractures if overloaded, and should maintain most of its strength up to 600oC. Design the material for this bracket, considering the various crystal imperfections as the strengthening mechanism.

Example 5.15 SOLUTION

In order to serve up to 600oC, the bracket should not be produced from a polymer material. Instead, a metal or ceramic would be considered.

Example 5.15 Design/Materials Selection for a Stable Structure

*

Example 5.15 SOLUTION (Continued)

*

*

Figure 5.24 The microstructure of BMT ceramics obtained by compaction and sintering of BMT powders. (Courtesy of H. Shirey.)

kT

Q

D

D

e

N

N

Recommended